Research Article of International Journal of Dental Research and Reviews
Color Stability of Different Resin Cement Systems: A Spectrophotometric Analysis
Rayan M. Eskandrani1, Roula al bounni2, Aead M. AlGarni3, Ayman M. AlGhamdi4
1Clinical Specialist in Restorative Dentistry, Department of Restorative Dentistry, Ministry of Health Riyadh, Saudi Arabia. 2Professor, Department of Restorative Dentistry, Faculty of Restorative Dentistry, Riyadh Elm University Riyadh, Saudi Arabia. 3Clinical Specialist in Restorative Dentistry, Department of Restorative Dentistry, Ministry of Health Khamis Mushait, Saudi Arabia. 4Clinical Specialist in Restorative Dentistry, Department of Restorative Dentistry, Ministry of Health, Al Baha, Saudi Arabia.
Aim: To evaluate the color stability of dual cure and light cure resin cements immersed in coffee solution at different time periods (baseline, 3 days and 1 week).
Materials and methods: The color stability of three light curing (Variolink Esthetic (VLC); Rely X Veneer (RLC) and Mojo Veneer (MLC)) and three dual curing (Variolink Esthetic (VDC); Rely X Ultimate (RDC) and Breeze (MDC)) resin cements were tested. A total of sixty disks (10 mm diameter and 0.5 mm thickness) were prepared using a silicone mold (n=10). The specimens were subjected to baseline color measurement using Commission Internationale de l’Eclairege L*a*b* (CIELAB) color space system with the help of a spectrophotometer (LabScan XE, HunterLab, VA, USA). Following baseline color measurements, the specimens were immersed in a staining coffee solution. The color measurement was repeated after 3 days and 1 week of immersion in coffee solution. All the data collected were statistically analyzed using repeated measures of Analysis of variance (ANOVA, P<0.05).
Result: After one week of storage in coffee solution, the mean color measurement scores in light cure group were found to be higher for RLC (1.22 ± 1.51) followed by VLC (0.85 ± 0.65) and NLC (0.68 ± 0.36) whereas in dual cure group, the mean color measurement scores were found to be higher for NDC (7.45 ± 4.50) followed by RDC (1.52 ± 1.24) and VDC (0.47 ± 0.34). Repeated measures ANOVA showed a statistically significant difference for light cure group (P=.004) at different time intervals but no significant difference with respect to dual cure group (P=.26).
Conclusion: There was a significant difference observed between the light- and dual-cured cements over a different period of time. The color changes of both light- and dual-cure resin cements were within clinically acceptable limits except for the dual-cured Breeze cement.
Keywords: Resin cement; Light cured; Dual cured, Ceramics, Luting, Cementation, CIELAB, Staining; Color stability
How to cite this article:
Rayan M. Eskandrani, Roula al bounni, Aead M. AlGarni, Ayman M. AlGhamdi. Color Stability of Different Resin Cement Systems: A Spectrophotometric Analysis. International Journal of Dental Research and Reviews, 2019, 2:21. DOI:10.28933/ijdrr-2019-06-2705
1. Ramos N, Luz J, Valera M, Melo R, Saavedra G, Bresciani E. Color Stability of Resin Cements Exposed to Aging. Operative dentistry. 2019.
2. Blackman R. Ceramic shade prescriptions for work authorizations. The Journal of prosthetic dentistry. 1982;47(1):28-35.
3. Brewer J, Akers C, Garlapo D, Sorensen S. Spectrometric analysis of the influence of metal substrates on the color of metal-ceramic restorations. Journal of dental research. 1985;64(1):74-7.
4. Imamura S, Takahashi H, Hayakawa I, Loyaga-Rendon PG, Minakuchi S. Effect of filler type and polishing on the discoloration of composite resin artificial teeth. Dental materials journal. 2008;27(6):802-8.
5. Arocha MA, Mayoral JR, Lefever D, Mercade M, Basilio J, Roig M. Color stability of siloranes versus methacrylate-based composites after immersion in staining solutions. Clinical oral investigations. 2013;17(6):1481-7.
6. Falkensammer F, Arnetzl GV, Wildburger A, Freudenthaler J. Color stability of different composite resin materials. The Journal of prosthetic dentistry. 2013;109(6):378-83.
7. Asmussen E. Factors affecting the color stability of restorative resins. Acta Odontol Scand. 1983;41(1):11-8.
8. Hekimoglu C, Anil N, Etikan I. Effect of accelerated aging on the color stability of cemented laminate veneers. Int J Prosthodont. 2000;13(1):29-33.
9. Nathanson D, Banasr F. Color stability of resin cements–an in vitro study. Pract Proced Aesthet Dent. 2002;14(6):449-55.
10. Peumans M, Van Meerbeek B, Lambrechts P, Vanherle G. Porcelain veneers: a review of the literature. J Dent. 2000;28(3):163-77.
11. .Kilinc E, Antonson SA, Hardigan PC, Kesercioglu A. Resin cement color stability and its influence on the final shade of all-ceramics. J Dent. 2011;39(1):15.
12. Braga RR, Cesar PF, Gonzaga CC. Mechanical properties of resin cements with different activation modes. J Oral Rehabil. 2002;29(3):257-62.
13. Hofmann N, Papsthart G, Hugo B, Klaiber B. Comparison of photo-activation versus chemical or dual-curing of resin-based luting cements regarding flexural strength, modulus and surface hardness. J Oral Rehabil. 2001;28(11):1022-8.
14. Santos GC, Jr., El-Mowafy O, Rubo JH, Santos MJ. Hardening of dual-cure resin cements and a resin composite restorative cured with QTH and LED curing units. J Can Dent Assoc. 2004;70(5):323-8.
15. Fradeani M, Redemagni M, Corrado M. Porcelain laminate veneers: 6-to 12-year clinical evaluation–a retrospective study. International journal of periodontics & restorative dentistry. 2005;25(1).
16. Khan AA, Siddiqui AZ, Syed J, Noori S. Spectrophotometric assessment of different surface coating materials on conventional glass ionomer cement. Pakistan journal of pharmaceutical sciences. 2016;29.
17. Da Silva DL, Mattos CT, de Araújo MVA, de Oliveira Ruellas AC. Color stability and fluorescence of different orthodontic esthetic archwires. The Angle Orthodontist. 2012;83(1):127-32.
18. Judd DB. Physiological Optics at the National Bureau of Standards. Applied Optics. 1967;6(1):13-26.
19. Archegas LR, Freire A, Vieira S, Caldas DB, Souza EM. Colour stability and opacity of resin cements and flowable composites for ceramic veneer luting after accelerated ageing. J Dent. 2011;39(11):804-10.
20. Vichi A, Ferrari M, Davidson CL. Color and opacity variations in three different resin-based composite products after water aging. Dent Mater. 2004;20(6):530-4.
21. Chang J, Da Silva JD, Sakai M, Kristiansen J, Ishikawa-Nagai S. The optical effect of composite luting cement on all ceramic crowns. J Dent. 2009;37(12):937-43.
22. Noie F, O’Keefe KL, Powers JM. Color stability of resin cements after accelerated aging. Int J Prosthodont. 1995;8(1):51-5.
23. Almeida JR, Schmitt GU, Kaizer MR, Boscato N, Moraes RR. Resin-based luting agents and color stability of bonded ceramic veneers. J Prosthet Dent. 2015;114(2):272-7.
24. Berrong JM, Weed RM, Schwartz IS. Color stability of selected dual-cure composite resin cements. J Prosthodont. 1993;2(1):24-7.
25. Ghavam M, Amani-Tehran M, Saffarpour M. Effect of accelerated aging on the color and opacity of resin cements. Oper Dent. 2010;35(6):605-9.
26. Mesbah A, Salah T, Sabet A. Assessment of color stability of different resin cements having different modes of polymerization before and after aging2016.
27. Koksal T, Dikbas I. Color stability of different denture teeth materials against various staining agents. Dental materials journal. 2008;27(1):139-44.
28. Ertas E, Gueler AU, Yuecel AC, Koepruelue H, Gueler E. Color stability of resin composites after immersion in different drinks. Dental materials journal. 2006;25(2):371-6.
29. Mutlu-Sagesen L, ErgÜN G, ÖZkan Y, Semiz M. Color stability of a dental composite after immersion in various media. Dental materials journal. 2005;24(3):382-90.
30. Palla E-S, Kontonasaki E, Kantiranis N, Papadopoulou L, Zorba T, Paraskevopoulos KM, et al. Color stability of lithium disilicate ceramics after aging and immersion in common beverages. The Journal of prosthetic dentistry. 2018;119(4):632-42.
This work and its PDF file(s) are licensed under a Creative Commons Attribution-NonCommercial 4.0 International License.